New Polymorphs of Ternary Sodium Tellurium Oxides: Hydrothermal Synthesis, Structure Determination, and Characterization of β-Na2Te4O9 and Na2Te2O6·1.5H2O.
Lee, Dong Woo; Ok, Kang Min; Inorganic chemistry 53 (2014) 10642–10648; doi:10.1021/ic501739u

data_4341561
_publ_section_title
;
 New Polymorphs of Ternary Sodium Tellurium Oxides: Hydrothermal
 Synthesis, Structure Determination, and Characterization of \b-Na2Te4O9
 and Na2Te2O6&#x00B7;1.5H2O.
;
_journal_issue                   19
_journal_name_full               'Inorganic chemistry'
_journal_page_first              10642
_journal_page_last               10648
_journal_paper_doi               10.1021/ic501739u
_journal_volume                  53
_journal_year                    2014
_chemical_formula_sum            'H6 Na4 O15 Te4'
_chemical_formula_weight         848.36
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90
_cell_angle_beta                 99.429(11)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.9884(19)
_cell_length_b                   14.3739(19)
_cell_length_c                   10.387(3)
_cell_measurement_temperature    298.0(2)
_cell_volume                     1323.9(5)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      298.0(2)
_diffrn_measured_fraction_theta_full 0.967
_diffrn_measured_fraction_theta_max 0.967
_diffrn_measurement_device_type  'Bruker SMART BREEZE'
_diffrn_measurement_method       CCD
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.06
_diffrn_reflns_av_unetI/netI     0.051
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            7741
_diffrn_reflns_theta_full        28.33
_diffrn_reflns_theta_max         28.33
_diffrn_reflns_theta_min         2.7
_exptl_absorpt_coefficient_mu    8.941
_exptl_absorpt_correction_T_max  0.82
_exptl_absorpt_correction_T_min  0.77
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details
; 
 SADABS(Blessing, 1995) 
;
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    4.226
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Block
_exptl_crystal_F_000             1488
_exptl_crystal_size_max          0.032
_exptl_crystal_size_mid          0.025
_exptl_crystal_size_min          0.022
_refine_diff_density_max         0.951
_refine_diff_density_min         -1.368
_refine_diff_density_rms         0.22
_refine_ls_extinction_coef       0.00027(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.954
_refine_ls_matrix_type           full
_refine_ls_number_parameters     120
_refine_ls_number_reflns         1600
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      0.954
_refine_ls_R_factor_all          0.0384
_refine_ls_R_factor_gt           0.0259
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0134P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0394
_refine_ls_wR_factor_ref         0.0417
_reflns_number_gt                1310
_reflns_number_total             1600
_reflns_threshold_expression     >2s\(I)
_cod_data_source_file            ic501739u_si_002.cif
_cod_data_source_block           Na2Te2O6(H2O)1.5
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to
/usr/data/users/saulius/crontab/automatic-downloads/current/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from
2011-04-26.

'_exptl_absorpt_correction_type' value 'EMPIRICAL'
changed to 'empirical' according to
/usr/data/users/saulius/crontab/automatic-downloads/current/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2827 2014-09-09 07:05:25Z andrius 
;
_cod_original_sg_symbol_H-M      C2/c
_cod_database_code               4341561